Gelatin as photosensitive material
Sergio Calixto 1, *, Nina Ganzherli 2, Sergey Gulyaev 3, Susana Figueroa-Gerstenmaier 4
1 Centro de Investigaciones en Optica, Loma del Bosque 115, Leon, Gto., c.p. 37150, Mexico; firstname.lastname@example.org
2 Ioffe Institute, St. Petersburg, Russia; email@example.com
3 Peter the Great St. Petersburg Polytechnic University, Russia; Gulyaev@rphf.spbstu.ru
4 Departamento de Ingenierias Quimica, Electrónica y Biomedica, Division de Ciencias e
Ingenierias,Universidad de Guanajuato Campus Leon, Loma del bosque 103, Leon 37150, Mexico;
* Correspondence: firstname.lastname@example.org; Tel.: +52-477-441-4200
Abstract: Because this issue journal is dedicated to Gelatin here we present a few applications of
gelatin in the field of optics. It is understood that optics is the science that studies the production,
propagation, interaction and detection of light. Regarding the detection there are some materials
sensitive to light (photosensitive) that are used like photomultipliers, CCD’s, crystals, two
dimension (2D) materials and more. Among the 2D materials the most popular through several
centuries has been gelatin based photographic emulsion that records spatial distributions of light.
More recently (1970) films made of Gelatin with Dichromate (DCG) and dyes have been used. We
describe some characteristics and applications of these two photosensitive materials. Also we
describe examples where gelatin is used as Relative Humidity (RH) sensor and in the fabrication of
optical elements based on gelatin. This article is intended to researchers outside the optics
Keywords: Gelatin; photosensitive materials; silver halide photographic emulsion; dichromated
gelatin; selective tanning; short-wave UV radiation; photodestruction; diffraction efficiency; dyed
gelatin; holographic structures; Weigert effect
Gelatin is a material that can be applied in many fields. For example in food (confectionery,
meats, bakery products, dairy products, beverages), health and nutrition (bone and joint health,
beauty, calorie management), pharmaceuticals (hard and soft capsules, vaccines, tablets, absorbable
hemostats), specialties (photographic gelatin, ballistics, lubricants, fuels, release agents, ignites), fats,
proteins and minerals (pet food, fertilizers, live stocks) and more .
Regarding the physics-optics fields, gelatin can be applied in the fabrication of photosensitive
materials. Undoubtedly the best known sensitive material is the photographic emulsion [2, 3]. Light
sensitive material in the emulsion is silver halide but it should be used with a binder that is gelatin.
Some others binders, like polyvinyl alcohol, have been used but the better is gelatin. Other
photosensitive material in the physics-optics fields is Dichromated Gelatin (DCG). Since its use in
the printing industry for over a century ago it has shown applicability. Perhaps the last successful
application is in the fabrication of holograms.
The photographic emulsion has been developed since the end of the 18th century. Many
researchers (amateurs and professionals), and companies have made contributions to the
development of photographic emulsions through the centuries. It is a theme that has been described
in many books, articles and more. Here in this article we just mention a few applications of gelatin in
photographic emulsion, DCG in holography, and fabrication of micro-optical components. This
article is devoted to researchers or people not acquainted with physics-optics. We give a brief
overview of the potential that has gelatin in the photosensitive materials. For those interested in
learning more details on specific themes can consult the references. Possibly they could gather more
information by using searching and databases engines (Google, Scopus, Optical society of America
OSA, SPIE, MDPI, Journals: Optics and Spectroscopy, J. of Optical Technology, etc.) and give the
word “gelatin” to the searcher. Besides the work done in the “western world” a great deal of
interesting researches have been developed in the former USSR. It is good to search those references,
for example [4-6]. More recently a Review of photosensitive materials for holography has been
published . Besides the gelatin based materials the review includes photopolymers,
photochromics, photorefractive, liquid crystals, and more.
Section 2 shows the use of plain gelatin films and gelatin mixed with colorants. Section 3
mentions the applications of gelatin as a part of the photographic emulsion and applications of it in
the fabrication of some optical elements. Section 4 describes the mixture of gelatin with dichromates
(DCG), the use of undeveloped DCG films, dyed DCG, Weigert effect in gelatin mixtures, DCG in
the fabrication of solar concentrators and more. In each theme we have mentioned some references
that show part of the work developed by different groups. We do not show all the references to
make this information manageable.
2. Plain gelatin
2.1. Gelatine chemical characteristics, fabrication process, environmental stability (pH, temperature, humidity)
Gelatin or gelatine is an important functional biopolymer widely used in foods to improve
elasticity, consistency, and stability. It is also used in pharmaceutical drugs, vitamin capsules,
photography and cosmetic industry. Gelatin is a protein made by the thermal denaturation of
collagen. It is colourless or slightly yellow substance. Commercially is available as a solid and
transparent, brittle, odourless and tasteless granule, sheets, flakes or powder, soluble in hot water,
glycerol and acetic acid, and non-soluble in organic solvents. Gelatin swells and adsorbs 5-10 times
its weight of water to form a gel. Gelatin forms a gel in water at a minimum concentration of 0.5%
and at pH range from 4 to 8 . Gelatin is widely used as a food ingredient and also is used as a
gelling agent forming transparent elastic thermos-reversible gels on cooling below about 35°C.
Additionally, due to its amphiphilic nature, it has emulsification properties as a foam-stabilizing
The source of gelatin from animals are hide and bone, and from vegetables are starch, alginate,
pectin, agar, and carrageenan, but their gels lack the elastic properties of the gelatin that comes from
animals. Gelatin is a mixture of peptides and proteins produced by partial hydrolysis of collagen
extracted from the skins, bones, tendon, and white connectivity tissues of animals such as
domesticated cattle, chicken, pigs, fish and even some insects. During hydrolysis, the molecular
bonds between individual collagen strands are broken down into a smaller molecules. Photographic
and pharmaceutical grades of gelatin come more often from cattle bones and pig skin [9,10].
Gelatin is a heterogeneous mixture of high molecular weight polypeptides and an important
hydrocolloid. It differs from other hydrocolloid because most of them are polysaccharide, whereas
gelatin is a digestible protein containing all the essential amino acids except tryptophan [11,12]. The
amino acid composition particularly with respect to proline and hydroxyproline can vary from
species, as a result of exposure to a wide range of environmental conditions, in particular,
As we already mentioned, gelatin is prepared by the thermal denaturation and physical and
chemical degradation of collagen. Collagen is the most abundant structural protein in both
vertebrates and invertebrates, and constitutes approximately 30% of an animal’s total protein.
Gelatin in a dry form consists of 98-99% protein. The molecular weight of these large protein
structures typically ranges from 20,000 to 250,000 g/mol, with some aggregates weighting in the
millions. The chemically structure of gelatin is described by a linear sequence of amino acids. It is
always written from the –NH2 end to the –COOH end by convention. The predominant amino acids
are glycine, proline and hydroxyproline. As a result, gelatin contains relatively high levels of these
amino acids: glycine 26-34%, proline 10-18% and hydroxyproline 7-15%. Other significant amino
acids are: alanine 8-11%, arginine 8-9%, aspartic acid 6-7% and glutamic acid 10-12%. The water
content will vary between 6-9%.
In gelatin manufacture, two methods are usually used: the acid and the alkaline processes (in
the pretreatment part) to produce type A and type B gelatins, respectively. In the acid one, pigskin
with an isoionic point of pH=7 to 9 is used. In an alkaline method, asparagine and glutamine
residues are converted to their respective acids and results in higher viscosity with isoionic point of
4.8 to 5.2 (pH). The functional properties of gelatin are related to their chemical characteristics. The
gel strength, viscosity, setting behaviour and melting point of gelatin depend on their molecular
weight distribution and the amino acid composition, the imino acids proline and hydroxyproline are
important in the renaturation of gelatin subunits during gelling. As a result, gelatin with high levels
of amino acids tends to have higher gel strength and melting point.
The criteria for good food-grade gelatins are not as demanding as those for photographic
gelatin. Viscosity and gel strength are the main physical properties for grading any gelatin under
carefully standardized conditions. Viscosity is determined at 60°C at a concentration of 6.67% (w/w)
air-dried gelatin. Gelatin forms gels similar to those of carbohydrates by forming a micro-structural
network. It is unique in that, at concentration as low as 1.0% it will form a thermoreversible gel. The
gel converts to a solution as the temperature rises to 30°C to 40°C, thus gelatin gels tend to melt in
the mouth. The melting point is the temperature at which a gelatin gel softens sufficiently and
allowing carbon tetrachloride drops to sink through it. Factors such as the maturing temperature
and the concentration of the gelatin gel tend to affects its melting point. The setting point of a gelatin
solution is dependent on its thermal and mechanical history. Higher setting temperatures are
encountered when the solution is cooled slowly in comparison to rapid chilling. Mechanical action
hinders or delay setting.
2.2. Gelatin as a mid-infrared recording medium
Gelatin is transparent to visible light. However, films with a thickness of about 90 µm only
show about 10% transmittance for mid-infrared light (λ= 10.6 µm). For thicker films mid-infrared
light is highly absorbed. This characteristic has been used  to fabricate surface relief gratings.
Thin films of gelatin having thicknesses from about 10 µm to about 50 µm were made and glued to
O-rings. Then they were placed in a two beam interference configuration which gives a sinusoidal
spatial intensity pattern. A CO2 laser was used (λ= 10.6 µm). These films recorded the sinusoidal
pattern. At the same time light from a He-Ne laser was sent to the recording area. It was found that
through exposure time relief gratings were recorded. First order intensity was monitored through
the exposure. Diffraction efficiency values of about 30 % were attained. These recorded gratings
were permanent. Their profile was studied with an interference microscope and resulted to be
sinusoidal. Besides the interference gratings, holograms were also recorded. The sensitivity of the
films resulted to be about some 1 J/cm2.
2.3. Gelatine as relative humidity sensor
We have seen in section 2.1 that gelatin is a complex chain of amino and imino acids linked
together in a partially ordered fashion by polypeptide bones. When water vapor is absorbed by
(desorbed from) the gelatin films its thickness changes. Film thickness will be minimum when the
film is dry and maximum when is swollen. When gelatin is dry its refractive index is about 1.5. But
when water vapor is absorbed by the gelatin its refractive index will diminish because the water
refractive index is 1.33. These thickness and refractive index changes can be detected with a
Mach-Zehnder interferometer. In reference  a method to measure Relative Humidity (RH) using
a gelatin thin film as sensor element is mentioned. They used thin gelatin films of about 24 µm glued
to an O-ring. To test the films a climatic chamber was used. In this chamber a Mach-Zehnder
interferometer was placed. A He-Ne laser was used as the light source. This interferometer
comprises two beams of light. One is called the reference and the other the testing beam. At the
output of the interferometer both beams are superposed forming a sinusoidal interference pattern.
The gelatin film is inserted in the testing beam. The RH in the chamber can be modified. Gelatin film
will respond to the changes in RH by changing its refractive index and thickness, as we have said.
These changes will make that the interference pattern present a lateral displacement. By using a light
point sensor it is possible to monitor the displacement. Thus we have a plot relating the intensity of
the interference pattern as function of RH. This is the calibration plot. Gelatin films could present
different physical characteristics that will affect the RH sensitivity of the films.
Besides the use of gelatin as RH sensor in a Mach-Zehnder interferometer, gelatin has been
used as the sensing element when optical fibers are used. In reference  is described a RH sensor
based on “single mode-multimode-single mode” fiber structure (SMS). The multimode fiber is
polished to remove the cladding, and part of the core, remaining a fiber structure with a “D” shaped
multimode profile. Then very thin gelatin layers are coated on the multimode fiber section by means
of the Dip Coating technique. They tested coatings with 3 and 6 layers. In the experiment one end
of the SMS was connected to a supercontinuum light source and the other to an Optical Spectrum
Analyzer (OSA). The SMS structure with the gelatin layers was placed in a climatic chamber where it
was possible to control temperature and RH. If RH raises gelatin refractive index decreases and the
losses in the light transmission will increase. By monitoring the losses for each wavelength from
about 1490nm to about 1510 nm we get plots of Transmission losses as a function of wavelength and
the parameter will be the RH. These are the calibration plots. A response time of 1 s was
mentioned. Besides the study just mentioned, reference  describe other application of gelatin
films together with optical fibers. For more information about gelatin applications with optical fibers
see the reference section of reference .
2.4. Gelatin with colorants (Dyed Gelatin)
We have seen that gelatin films transmit well light with wavelengths between 400 nm to about
800 nm. Thus, to make gelatin films sensitive to visible light a dye should be added. This process was
exposed in reference  by the group of Prof. Sirohi where they mention the use of an organic eosin
dye embedded in thin layers (8 µm) of gelatin. Eosin dye belongs to the family of xanthene dyes.
They recorded sinusoidal interference patterns (λ= 532 nm, Nd:YAG laser) with a period of 5.7 µm.
The result was the formation of surface relief gratings. When studied with an Atomic Force
Microscope these gratings showed a sinusoidal relief. The depth of the relief was about 70 nm for
gratings having 3% diffraction efficiency (DE).
Another study that comprised the use of dye incorporated in gelatin is described in references
 and  by the group of Prof. Pantelic. There, they describe a mixture of gelatin, tot’hema and
eosin to render gelatin sensitive. Tot’hema is a drinkable solution used in medicine for curing
anemia. Eosin is an organic dye used in medicine too. It shows a maximum absorption in the green
part of the spectrum. Gelatin layers were fabricated by the gravity settling method. 100 µm thick
layers were made. A Nd:YAG laser was used to make negative microlenses. They showed parabolic
profiles. The process to form the lens is thermal. Radiation from the laser is completely absorbed by
the film. As energy is absorbed an increase in the layer temperature is present until it reaches the
gelatin melting point. At this stage the gelatin becomes liquid. By thermocapillary forces the liquid
flows and the formation of a dip is present.
The recording of holograms considers the interference of two light beams, one that comes from
the object (object beam) and another one called reference. Here it is supposed that both beams have
the same linear polarizations which is perpendicular to the plane of incidence. However, object
beam could present any polarization state, i.e. linear, circular or elliptical. Thus a recording medium
capable of recording the polarizing pattern should be used. Once the recording is done the hologram
is illuminated with the reference beam and the object beam is generated. It will present the same
polarization state that light coming from the object had. This is called polarization holography. The
group of Prof. Ebralidze (Georgia) [19-23] developed a technique where they used dyed gelatin to
record polarizing holograms. Azo-dye-colored gelatin films (methyl-orange, methyl-red, and other
dyes) were prepared on glass plates. Then they were illuminated with a mercury lamp. This light
induced anisotropy. Light is absorbed by the dichroic molecules whose axes are oriented along the
polarization vector. These molecules become centers of photoinduced crystallization. The grain
concentration is proportional to the light intensity. They developed theory and experiments. In
references [19-23] are mentioned some articles of the group but they published more information.
3. Gelatin in the photographic plate (mainly holography)
3.1 Photographic plate in holography.
In 1674 Christoph Baldwin produced calcium nitrate by highly heating a mixture of chalk and
nitric acid . After drying the mixture he found that the mixture was luminous. He called the
mixture “Phosphorus” (carrier of light). Later in 1721 Heinrich Schulze attempted to reproduce
Baldwin’s experiment. At one time he made a mixture containing nitrate of silver, chalk and nitric
acid. He though this will dissolve chalk. When, after heating, he exposed accidentally this silver
mixture to light he noticed that silver salts were sensitive to light. He discovered the sensitiveness to
light of the silver salts. Later the based silver salts photosensitive wet plates were proposed to record
images (Daguerrotypes). In 1850 Poitevins did the first experiments that used gelatin as a binding
element for silver salts to make sensitive emulsions but were unsuccessful. Until 1871 Maddox
mentioned the use of gelatin as a binder for the silver bromide emulsions. This was the first
successful dry emulsion made with gelatin silver bromide.
In the photographic plate three silver halides can be used: silver chloride, silver bromide and
silver iodide. Some of them give more sensitivity to the plate. Grain sizes vary from about 10
nanometers to a few micrometers. The sensitivity of the plate can go from the ultraviolet light to the
green part of the spectrum depending on the mixture of silver halides. By adding dyes it is possible
to cover the visible spectrum and infrared ligth. For a more in-depth description of the photographic
plate fabrication, sensitivity,characterization, emulsion structure and more, the reader could consult
the references [2, 25].
Through some centuries the photographic emulsion was used to record mainly photographs
and radiographies. Much scientific work was developed to offer very good photographic plates.
However, when holography was developed by Dennis Gabor, in 1948, new mixtures of the
photographic emulsion were fabricated. Holograms are made by recording interference light
patterns. These patterns are produced when light from an object interferes with other beam called
reference beam. These beams are coherent. They usually interfere at an angle. The number of
interference lines could be between about a few lines per millimeter (l/mm) to about 5000 l/mm.
Thus, new studies were made to find silver halide emulsions that fulfilled the requirements of
holography. Among those requirements the recording medium should present high sensitivity,
high spatial resolution, linearity in response, low noise, this implies that that the material should not
present grain structure, if there are grains they should be small, availability in different formats, low
cost and long term stability. Several references mentioned the available commercial emulsions at
that time (1970) and later [25-30]. Unfortunately some of those emulsions are not produced anymore.
In these days (2018) one supplier of photographic papers and holographic plates is Slavich .
It has the following emulsions: PFG-01 (red sensitive plates and films), PFG-03M (red sensitive
plates), PFG-03C (panchromatic plates and rolls), DCG plates (Blue green sensitive, PFG-04), VRP-M
and VRP silver halide plates (green sensitive).
At present (2018) a few groups make studies of the actual silver halide plates. One is the group
of Prof. Belendez in Alicante, Spain. They have made different studies of the PFG-01 and the BB-640
plates [32-34]. More references to their work can be found. Other group is in Saint Petersburg
National Research University of Information Technologies, Mechanics and Optics (ITMO), St.
Petersburg, Russia . They have studied new visible light optical sensitizers for PFG-03 plates.
Regarding the use of silver-halide plates when near-infrared and mid-infrared light is used a
study  shows that by the use of triethanolamine and a thermal cycle it is possible to extend the
sensitivity range of silver halide plates to record light having a wavelength of 1.7 µm. Other study
 shows the use of silver halide films using light with a wavelength of 10.6 µm. See the references
therein to find more information about the use of silver halide films with infrared radiation.
3.2 Short Wavelength Ultraviolet Method (SWUV) used to fabricate holographic structures
Gelatin is the main component of the two most common photosensitive media used in optics
(comprising holography): silver halide photographic emulsions and layers of Dichromated Gelatin
(DCG). Therefore the efforts of researchers in the holography field have been aimed to the
development of methods that change the physical-chemical properties of gelatin in accordance with
the recorded interference pattern. Gelatin processing methods involve two main types of effects:
selective structuring and destruction of gelatin molecules. When they are applied, separately or
together, they give rise to a variety of methods in the fabrication of high performance phase
holographic structures on gelatin-containing photosensitive media.
The formation of the phase holographic structure is associated with the “development” – an
operation that allows the modulation of the physical and chemical properties of gelatin. There are
two kinds of the development: equilibrium and non-equilibrium. The non-equilibrium
“development” involves the selective structuring (tanning) of the gelatin layer. When silver halide
plates are used they suffer the tanning changes through the bleaching chemical process. However, if
DCG is used the process is done photolytically. In both cases the non-equilibrium “development” is
done by the rapid dehydration with isopropanol of the gelatin layer. This includes the method of
creating “microcavity holograms” [38, 39] and the Silver Halide Sensitizing Gelatin method (SHSG)
[40, 41]. The non-equilibrium development methods are extremely sensitive to the processing
conditions and the type of silver halide photoemulsion or DCG used. The application of these
processes allows the fabrication of purely phase volume holograms.
3.2.2. The SWUV method among other methods of obtaining phase holographic structures
The equilibrium “development” is associated with the slow drying of a gelatin layer in the air.
This means that the use of isopropanol is not required. Equilibrium development methods are
associated with either selective tanning, when silver halide emulsions are bleached , or selective
gelatin photodestruction of the gelatin-containing sensitive media [43, 44]. When these processing
methods are applied good results are obtained regardless of the type of the gelatin containing
sensitive medium and processing parameters. The application of these methods allows the creation
of purely phase relief holographic structures.
The formation of the surface relief during selective tanning of silver halide photoemulsion is
due to the tension forces arising in the process of the photoemulsion drying. The redistribution of
gelatin leads to the formation of crests of surface relief at tanning areas, i.e. at the areas with the
greatest density of a Silver Image (SI) (Figure 1a) .
(a) (b) (c)
Figure 1. Creation of surface relief (a) during selective tanning and by destructive effect of UV radiation (b) on
silver-halide photoemulsions and (c) on layers of DCG.
As an organic substance, gelatin absorbs UV radiation well. This is the basis for the method of
the destructive action of short-wave UV radiation, with a wavelength less than 250–270 nm, on
gelatin (SWUV method) of the silver halide photoemulsion . In this case, the primary SI serves as
an effective screen that modulates the intensity of the UV radiation. The destructive effect of UV
radiation leads to breaking main bonds in long chains of gelatin macromolecules and their
fragmentation and solubility in aqueous solutions (see Figure 1b).
In the case of DCG, the physical-chemical properties of gelatin are changed directly by the
holographic recording of the interference pattern due to selective laser light tanning in the presence
of dichromates (Figure 1c) . Thus, a structuring takes place, i.e., the creation of a large number of
cross-links in the maxima of an interference pattern. A large number of cross-links prevents the
fragmentation of gelatin macromolecules under the effect of UV radiation and their dissolution in
water. Thus, the crests of the surface relief after the water procedure are formed in the maxima of the
interference pattern. Both main effects on gelatin: selective structuring and destruction, are
consistently applied for the formation of a phase hologram on DCG.
All the methods of creating relief-phase holographic structures by means of the equilibrium
type of the development allow one to obtain a significant depth of the surface relief in the range of
spatial frequencies up to hundreds of lines/mm (l/mm).
3.2.3 Regular holographic structures obtained by the SWUV method
The DE of relief-phase structures obtained by holographic methods is largely determined by the
height (depth) of the surface relief h measured as the total difference between the crests and valleys.
Since the range of recorded spatial frequencies does not exceed several hundreds l/mm, the
diffraction of light can be described by the Raman-Nath approximation . According to this
approximation, the DE η1 of a transmission structure with a sinusoidal relief profile, in the first
diffraction order, can be represented as:
where the amplitude of the phase modulation of the illuminating beam is in the argument of the
Bessel function J1. The square of the Bessel function becomes the maximum value of ~ 0.34 when the
value of its argument is approximately equal to π/2:
Since gelatin has a refractive index n0 close to 1.5, then the height of the surface relief h, providing a
maximum intensity value of the first diffraction order, is approximately equal to λ. This value can be
considered as the criterion for the surface relief depth that is necessary for the effective diffraction of
the regular periodic structure.
Table 1 presents the main parameters of the regular holographic structures on silver halide
photoemulsions of different types and DCG layers, created in the laboratory, by the SWUV method
[43, 44, 46-50].
Table 1. Parameters of the regular holographic structures on silver halide photoemulsions and DCG.
of the height
of the relief
efficiency η1max, %
for λ = 0.6328
14 - 18 Fresnel zone plate 0 – 57 l/mm
1.2 – 2 34
2Photoplates VRL 14 - 18 grating
3Photoplates VRL 14 - 18 grating
7 grating 65 l/mm
7 microlens array
2.6 – 2.8 -
6 - 7 grating 40 l/mm
5 grating 130 l/mm
5 grating 130 l/mm
(Kurchatov Institute of Atomic Energy),
1.8 grating 130 l/mm
10DCG layer 51 - 86 grating
1.35 – 1.45 25
11DCG layer 0.6 – 1.1 grating
0.6 – 0.9 28 - 30
from the DCG layer to the PMMA
0.3 - 5 grating 103 l/mm
0.48 – 1.3 8 - 25
As can be seen from the Table 1, a large value of the depth of the surface relief provides a high DE of
regular structures, approaching the theoretical limit for thin phase holograms. This indicates the
possibility of creating high-performance regular holographic transmission structures for the visible
and near-infrared light spectrum.
3.2.4 Random phase structure obtained by the SWUV method
The determination of the required depth of the surface relief for random holographic structures
(diffusers) is somewhat different than the one presented in the preceding section. For practical
applications of random structures, it is necessary to ensure a minimum proportion of the
non-scattered light component (zero diffraction order) that passes through the diffuser. According to
the theory of light scattering on large-scale inhomogeneities in the Kirchhoff approximation, if the
distribution of the relief height is described by the Gaussian function , the amplitude reflection
coefficient of the non-scattered component is equal to:
where k = 2π/λ is the wave number, λ is the wavelength of light, σ is standard deviation of the relief
height and ψ is the slope angle of the beam. For transmission structures  at ψ = 90°, formula (2) is
where η0 is the relative intensity of a zero order beam as a percentage of the incident beam, n0 is the
mean refractive index of gelatin equal to 1.53 (for λ = 0.6328 µm). The small values of the relative
intensity of the non-scattered component, for example, η0≤ 0.1%, are achieved with values of the
standard deviation of the surface relief height σ ≥ 0.5 µm. The last inequality can serve as the
criterion for the efficiency of the transmission scattering structure.
Table 2 presents the main parameters of holographic diffusers obtained on PFG-01 plates when
using the SWUV method . The SWUV method is able to provide the value of the standard
deviation of the surface relief height (sample 1), which is necessary to achieve the low value of the
intensity of scattered light components η0. The low values η0 (samples 2, 3) can be also obtained at
the values of standard deviation σ that are significantly lower than the values required by the
theory. This can be explained by the fact that some samples may maintain certain regularity in the
structure depending on the way the diffusers are produced.
Table 2. Parameters of holographic diffusers.
The average thickness of the photographic
emulsions after processing by the SWUV
σ, μm hmax,
for λ = 0.6328 μm
11.4 0.54 1.9 0.12
22.4 0.36 1.5 0.079
33.4 0.41 1.8 0.057
Thus, the SWUV method proved to be applicable for the creation of efficient random and
pseudorandom structures such as narrow directed diffusers operating in the visible spectrum range
3.2.5. Creation of a large depth surface relief and the phenomenon of the structure period doubling
The effective absorption of the short-wave UV radiation by gelatin is limited to a narrow
near-surface layer due to the strong self-absorption of gelatin . Thus, the photodecomposition of
gelatin, and its transformation into a soluble state, is a purely surface process covering only the
depth of 1 - 2 µm of the total thickness of commercially produced photolayers that is equal to 5 - 18
µm. Therefore the required original thickness of the silver halide photographic material can be
significantly reduced. For example, high values of DE η1 can be obtained when SRBSh
photoemulsions are used (Table 1, #9). This emulsion has a thickness of T=1.8 µm.
There are some applications where the holographic structures should present significantly
larger surface reliefs than the ones given in Table 1. These applications comprise the use of structures
working with infrared light, structures that should present higher diffractive orders, or structures
that can be used as a mold to transfer their holographic characteristics to other substrates. The
repetition of the treatment cycle “UV radiation – washing – air drying”, for the VRL photoemulsion,
allowed us to increase the height of the surface relief h at low spatial frequencies (ν≤ 30 l/mm) up to
the values of 5 - 8 µm. In the places with the lowest SI density it is possible to obtain “windows”
where the layer thickness tends to zero . That is, there is no gelatin in those places. However, in
the area of higher spatial frequencies (ν > 40 - 60 l/mm), a very interesting physical phenomenon was
discovered: the doubling of the period of the holographic structure (the formation of spatial
subharmonics), Fig. 2 . The significant increase of the total UV exposure time and the number of
repeated dryings generate two processes: the destruction in the places with the lowest density of SI
and the photostimulated tanning (structuring) in the same places. As a result, the holographic
structure loses the stability. The tension forces initiate the pairwise union of neighboring relief crests
and the violation of the spatial symmetry of the structure. A similar example of the spatial
self-organization and formation of domain structure caused by the instability of the thermodynamic
system is present in the field of dynamic holography when photorefractive crystals are used .
Fig. 2. Microphotograph of holographic Fresnel Zone Plate, including the area with period doubling.
The phenomenon of period doubling, when ultra-deep reliefs are obtained, can be avoided if a
multi-cyclic treatment is replaced with continuous aqueous etching of gelatin while irradiating
samples with a mercury lamp .
3.2.6. SWUV method and ultra-thin DCG layers
The concept of the surface action of short-wave UV radiation on gelatin is quite applicable to
the layers of DCG. Instead of the modulation of the intensity of UV radiation by a SI, we have here a
variable layer tanning (Figure 1c), that modulates the destructive effect of short-wave UV radiation
on gelatin in the upper layers. A significant decrease in the thickness of the DCG layer (Table 1, # 11,
12) [49, 50] up to the values of the order of λ provides high values of the DE η1 that are close to the
theoretical limit for thin holograms. In the case of ultra-thin DCG layer (T < 1 µm), for a sufficiently
long UV irradiation time, gelatin-free “windows” appear. Multiple repetition of the cycle “UV
radiation – washing – air drying” for the layers with the thickness T < 3-6 µm leads to the same
result. This fact allowed one to realize the effective transfer of holographic relief structures from the
DCG layer onto a PMMA substrate . In this case the sequential application of the DCG treatment
and the resists processing are used (Table 1, # 12).
3.3 Other applications of the photographic plate
Nowadays (2018) the photographic plate has been replaced as light sensitive material by CCDs
and other electronic devices. However, photographic emulsions are applied in fields like recording
of landscapes and portraits, motion pictures, aerial photography, microfilm, traffic and surveillance,
nuclear physics and more. For more information of the actual commercial emulsions please consult
the web pages of Kodak, Agfa-Gevaert, Fujifilm, Ilford and Slavich companies to mention but a few.
The photographic plate can be used to make relief micro-optical elements. By pure relief is
meant that there are variations in the height of the gelatin. Altman  mentioned that when
common developers were used the height of the relief image on the plate was of the order of 1 µm
when the silver density was 4.0. But still higher relief images were generated when tanning bleach
was used. Relief images higher than 3 µm were obtained. Other studies mention the use of PE-2
photographic plates . Based on this method it is possible to fabricate relief surface zone plates
 and microlenses .
Cloud chambers and bubble chambers have been used for visualizing the passage of ionizing
radiation. The discoveries of the positron (1932) and the muon (1936) were done with cloud
chambers. These chambers use photographic emulsions. More recently an experiment was done to
detect Tau neutrinos originated from Muon neutrinos [62-65]. Protons were generated at the CERN
facilities (Switzerland) and sent to carbon targets which produced pions and kaons. They decay to
produce muons and neutrinos. To find the decay of Muon neutrinos into Tao neutrinos a special
chamber was built in Italy, 730 km away. This consisted of an Emulsion Cloud Chamber (ECC) 10 m
x 10 m x 20 m. The name of the project was Oscillation Project with Emulsion-tRacking Apparatus
(OPERA). The basic ECC unit of OPERA detector is a brick that consists of a sequence of 57 emulsion
photographic films interspaced with 56, 1 mm thick lead plates, packaged in a light tight container.
The brick weights 8 Kg and have a thickness of 7.5 cm. The total number of bricks is 154 000 giving a
total number of 10 million nuclear photographic films. These special films are made by Fuji Film co.
Each film is made of two 44 µm thickness sensitive layer separated by a 205 µm thickness plastic
base. The size of the grains in the photographic nuclear emulsion is between 0.1 µm and 0.5 µm. A
detailed explanation of the nuclear photographic emulsion is given in reference . See also the
4. Dichromated Gelatin (DCG)
4.1 DCG characteristics and sensitivity (UV and visible light)
A dichromated colloid consists of an organic colloid dissolved in a solvent that is usually water.
To this solution a chromate or dichromate is added. They form photosensitive layers. Among the
sensitizers are, for example, ammonium dichromate, potassium dichromate and sodium
dichromate. All chromium compounds are poisonous. They can be absorbed through the skin and
act as a protein precipitant. Photosensitive organic colloids can be divided in two general groups,
proteins and carbohydrates. Gelatin, animal glues, albumin, casein, and others belong to the first
group. Gum Arabic and starch belong to the second group. The compound of gelatin and
dichromates (DCG) is the most used in optics. When the colloid is exposed to light the colloids are
hardened. In the dichromated colloids the photosensitive component, the dichromate, absorbs
efficiently ultraviolet, violet and blue light. Maximum absorption is at a wavelength of 367 nm.
Factors that affect the sensitivity are the dichromate concentration, value of the pH, layer thickness
and moisture content, for example. A detailed description of dichromated colloids can be found in
4.2 Undeveloped DCG
4.2.1 Real time use of DCG
Holograms and diffractive elements made with DCG present very good diffraction efficiency.
However, after the recording step DCG plates should be developed and this is a drawback because it
takes time and plates should be displaced out of the recording configuration. There are holographic
materials that can be used in real time but they are expensive, like the photosensitive crystals.
However, it has been shown that DCG can be used in real time. DCG responds efficiently to
ultraviolet (UV) and blue-green light. But it is almost insensitive to red light. Thus the recording step
can be made with UV-blue-green light and the reconstruction in real time can be done with red light.
For example using light from a He-Ne laser. The characterization of DCG working in real time was
exposed in reference . Diffraction efficiencies of about 0.2% were found. Gratings spatial
frequencies ranged between a few hundreds to above 1000 l/mm. Applications in the fields of
interferometry, object edge enhancement, character recognition, image subtraction, and phase
conjugation were presented.
Further studies of DCG plates used in real time were shown in reference . They developed
theory that predicted the behavior of diffraction efficiency as a function of time of exposure. The
recorded gratings resulted to be pure absorption gratings. This phenomenon was present whenever
the exposed plate remained in an environment with the same relative humidity with which the
gelatin was sensitized, dried and exposed. However, when recorded absorption gratings were
stored in an atmosphere with higher humidity a phase grating with more diffraction efficiency was
4.2.2 Thick-layered self-developing dichromated gelatin for volume hologram recording
Two types of self-developing photosensitive materials, based on DCG, for real time volume
hologram recording were created. The developing process of a hologram recorded in DCG requires
some quantity of water. In one case, we produced a sandwich structure in which dichromate gelatin
is found between two glass plates . We call this layer “gel-like”. The process of layer
manufacture was similar to the well-known technology of DCG . The major difference is that the
hologram is recorded directly in the moisture-saturated layer. The layer itself is a rather dense gel
with a thickness ranging from 1 mm to 5 mm. The hologram can be recorded as easily as with a solid
In another case, the self-developing glycerol-containing dry layers of DCG, with a thickness of
70-400 µm, were produced and studied . Similar layers with a small thickness of 1-5 µm were
described earlier in . Glycerol serves as a plasticizer and is used to hold a certain amount of water
molecules. These molecules are involved in the development of latent image due to the presence of
hydrogen bonds. A hot solution of DCG with the addition of glycerol was poured on a glass
substrate. The layers were gelled in a refrigerator for a day and then dried for several days at the
room temperature. As a result, their thickness decreased by a factor of 5-6.
The main holographic parameters of the layers, “gel-like” and “glycerol containing”, were
determined by recording holographic gratings using the symmetric scheme. The He-Cd laser (λ=442
nm), with a power of 16 mW, was used as a light source. Holographic parameters of the gratings in
DCG layers containing glycerol are better than those of the gel-like DCG. The maximum attained DE
was 15-40% depending on the layer thickness and ammonium dichromate concentration. The
sensitivity of a thick-layer glycerol-containing DCG is equal to about 6-10 J/cm2, which is close to the
sensitivity of thick-layered gel-like gelatin (10 J/cm2). The thick-layered DCG containing glycerol is
characterized by a virtually endless storage time for recorded holograms unlike the gel-like DCG
that had the smallest lifetime of the recorded information (several hours). The main applications of
the above-mentioned DCG volume media operating in real time are described in .
More studies of the mixture DCG, glycerol and methylene blue were done [74-75]. They
characterized the films finding the optimal relation of glycerol and gelatin. The addition of glycerol
decreased the achievement of the maximum diffraction efficiency.
4.3 DCG used to make relief lenses and gratings
DCG is usually used to make phase elements, that is, modulation of the bulk is the base.
However, it can be used to make relief optical elements like lenses and diffraction gratings. In
reference  is mentioned the method to make microlenses and micromirrors. Unhardened layers
with a thickness of about 8 µm were used. The optical recording configuration comprised the use of
a white light source, a mask and a lens. The mask consisted of holes with different sizes. An image of
the mask was formed over the DCG layer. Diameter of the holes images ranged between several
hundred microns to some millimeters. Thus, this is a lithography method. After the recording, layers
were developed with water and alcohol. At the end of the process relief microlenses and
micromirrors were present. They were investigated with an interference microscope. The sagita
value was about some microns. Lenses presented focal distances of some milimeters. Different types
of masks were studied. Some had holes, as we have mentioned, others rings (annular design) and
also masks with parabolic transmittance. When this last mask was used, the lenses gave the best
image. Also array of microlenses were made by interference of three beams. These beams were not in
the plane of incidence
To commercialize holograms it is common to copy the relief of master holograms on different
polymers. This copy process is called embossing or casting. A study was done to find if the master
holograms could be made with DCG . To characterize the DCG film, interference gratings with
different spatial frequencies were recorded. DCG plates had a thickness ranging between 0.7 µm and
0.8 µm. Films were made by incorporating ammonium dichromate in a 2% gelatin solution. A He-Cd
laser was used. After the exposed gratings were recorded the DCG plates were washed in water, the
unhardened regions were dissolved and a relief grating appeared. It was found that DCG layers,
show very low scattering but its spatial resolution fell when the spacing between fringes was in the
order of a few microns.
The relief enhancement of recorded holograms can be made by means of biochemical etching.
In reference  they used a proteolytic enzyme called Papain dissolved in water. Diffraction
gratings on DCG were fabricated by contact-copying Ronchi gratings. These gratings consists of
transparent and opaque strips with low spatial frequencies (0.25 l/mm). After the recording and
developing steps they immersed the plate in a solution containing papain from 0.1 to a few units of
%. They found that the relief depth was increased. Diffraction efficiencies rose. However, when
gratings were made by recording a sinusoidal interference pattern, using an argon laser, the results
were not so positive, spatial frequencies varied from 500 l/mm to 1500 l/mm. Besides this research
with papain it seems in reference  they also used biochemical etching but the biomaterial is not
4.4 Dyed DCG
As we have seen above the spectral sensitivity of DCG is limited to light with wavelengths less
than about 540 nm. In the early 70’s efforts were made to sensitize DCG films to red light [80, 81].
One of those references mentions the use of thiazine and triphenyl methane family dyes. The former
dye precipitated in the presence of ammonium dichromate solutions. The last family of dyes showed
better compatibility with dichromate solutions. Used dye was Acid Fast Violet BG (AFV). They
tested the DCG Dye sensitized plates to record gratings with 815 lines/mm and 1000 lines/mm and
found a maximun diffraction efficiency of about 30% for layers having 6 µm thickness and about
50% for layers 20 µm thickness. A better method to sensitize DCG layers was proposed by Prof.
Kubota [82-89] in 1976. He used methylene blue (MB) as sensitizer. In the first reference he shows the
practical method to prepare DCG-dye layers. He found that the absorption spectrum of MB
sensitized plates showed an absorption band at 372 nm, due to the ammonium dichromate, and
other two absorption bands were present at 620 nm and 670 nm that were due to the MB. 90% of
light with 633 nm wavelength was absorbed in a 20 µm thickness layer. After testing the plates he
found a diffraction efficiency of about 88% for gratings having 1050 l/mm. Energy required to
achieve these efficiencies was 150 – 400 mJ/ cm2. This energy is about 10 times the needed for
conventional or DCG plates with no dye.
More studies and applications of MB dyed DCG were made besides the studies made by Prof.
Kubota. For example Changkakoti [90-92] made systematic studies to investigate the influence of
various relevant chemical and physical parameters on the diffraction efficiency of MB sensitized
DCG plates. He studied: a) the pH dependence of the developer, b) the role of the external electron
donor and c) their storage life and processes of MB sensitized DCG plates. After him a study
presented a new electron donor . It was found that tetramethylguanidine (TMG) produced
bright holograms when exposures in the order of 50 mJ/cm2 were given. Other study  mentions
the role of the ratios and concentrations of prehardener, fixer and sensitizing solution as well as pH
dependence and storage time.
Besides MB with dichromates other dyes of the xanthene group have been tested to record
interference gratings. A study  mentions the use of Rhodamine 6G and Erythrosin B. A He-Ne
laser giving light with a wavelength of 543 nm was used for the recording. It was found that
sensitivity with these dyes was better than just DCG at the mentioned wavelength.
4.5 Weigert effect in gelatin films
In this section we will describe the formation of anisotropic plates that show the Weigert effect.
Plates based on gelatin can be photographic emulsions, DCG-dye plates or just dyed gelatin plates.
Suppose that we have a silver halide emulsion and it is illuminated by natural white light until
saturation occurs. Then it is developed to transform the silver halide into metallic silver. After this
the plate is bleached and the opaque metallic silver is converted into a transparent silver-chloride
emulsion. Then the plate is illuminated with a strong linearly polarized light. During the exposure
the illuminated areas will darken due to the instability of the bleached silver halide. If after the
exposure we place the plate between crossed polarizers the illuminated areas will behave as a
uniaxial (dichroic) medium. This phenomenon was described by F. Weigert in 1919 and it is known
as the “Weigert effect.”
In a series of papers [96-102] Jonathan and May have exposed the results of experiments when
they used silver-chloride plates. For example they recorded two images in a silver-chloride plate.
Then they observed the plate between crossed polarizers. This allowed a separate restitution of any
of the two images. Another example is given when a transparency is placed in contact with the
silver-chloride and illuminated with polarized light. Then the plate is placed between crossed
polarizers and the image of the transparency is shown with its polarity. However, if the analyzer is
rotated the birefringent parts will turn blue and the non-exposed ones will be white giving an
appearance of a contrast reversal. Also with this method they found the diffeence between two
The photoanisotropy phenomenon or Weigert effect can also be obtained with dyed
dichromated gelatin layers. This application was shown by Prof. Kakichashvili in a series of papers
[103-107]. He used dyed-DCG plates. At the beginning he used blocks that had embedded a
photochromic substance, Trimethylspiranebenzopyran. He illuminated them with He-Ne polarized
light and then he bleached them. He observed a photoanisotropy effect. He used this phenomenon
as the basis of what he called Polarization Holography. That is, the recording of intensity, phase,
wavelength and polarization of an object wave when interferes with a reference wave. In
reconstruction the object field together with its polarization is obtained. Later he proposed another
photosensitive medium that was DCG with dyes. He mentioned the use of dyes of the
triphenylmethane group. Some of them showed the capacity to produce the photoanisotropy or
Weigert effect. Anisotropy was detected when samples were introduced in a polariscope. More
recent applications of the Weigert effect are mentioned by Wardosanidze in reference . Other
group that intensively worked in polarizing holography was leaded by Prof. Todorov [109-112].
They began using KCL:Na material containing Fa centres. Later they used mixtures of dyes and
polymers. Another material that they developed, also based on gelatin, was mentioned in a patent
. There they mention the use of Arsenous sulphide (As2S3) dispersed in gelatin. Later they
exposed a characterization  of the mixture where they show that dyed gelatin plates show an
absorption edge shift when they were illuminated with linearly polarized light. More information
can be found in reference .
Among the dyes mentioned by Kakichashvili was malachite green. Later more studies using
this dye were presented in references [116-121].
4.6 DCG in holographic solar concentrators
Holograms can be made to display images or to behave as optical elements. Among the optical
elements are the lenses. In the case that a hologram behaves as a lens it is called hololens. It can focus
light or form an image. However, because holograms are based on the diffraction phenomenon if
light with different wavelengths reach the hololens each wavelength will be focused in a different
If an object is placed outside the optical axis of an ordinary lens its image will be also outside
the optical axis. This characteristic can also be presented by the hololens. It can be fabricated so as to
work as an off axis element. Thus, light that comes from a distant object will be focused outside the
Light that comes from the sun can be considered as direct o diffuse. Sunlight presents many
colors or wavelengths. Its spectrum is centered in the yellow part. The range of wavelengths in the
solar spectrum mainly goes from about 0.3 µm to more than about 1.3 µm. This light can be
converted to electricity by Photo Voltaic cells (PV). Each kind of these cells responds better to a
certain range of wavelengths. Among the cells there are the ones made of Indium Gallium
Phosphate (InGaP) and the ones made of Silicon (Si). The formers respond to wavelengths from
about 0.3 µm to about 0.7 µm with peak absorption at about 0.65 µm. The last ones show a range
from about 0.3 µm to about 1.1 µm with peak absorption at about 1 µm.
Here we describe briefly a holographic solar concentrator . A compound holographic solar
concentrator has been built and comprise several modules. Each module consists of two off axis
hololenses and three PV cells in the configuration: Si-InGaP-Si.
Hololenses have been fabricated with DCG. The behavior or response of the hololens in relation
to the wavelength is as follows. Light with a wavelength of 850 nm and higher wavelengths are
transmitted without deviation through the hololens to a silicon PV cell that is behind the hololens.
Light with a wavelength of about 500 nm or a little higher is sent to the InGaP cell that is off axis of
the lens. With this method the efficiency of the concentrator was 19% higher when compared to the
more efficient cell system based only on Si cells.
Other optical configurations of holographic solar concentrators and related matter can be found
in references [123-125].
4.7 Display Holography
The history of intensive application of gelatin-containing photosensitive media in holography
has been developed for more than fifty years, beginning with the pioneering works of Yu.N.
Denisyuk  and E. Leith and Yu. Upatnieks . They proposed methods of recording volume
and transmissive holograms on silver halide photographic emulsions.
Gelatin-light sensitive materials in holography have been applied to fabricate displays used in
industry, engineering, medicine, energy, education, advertising, metrology, microscopy,